Poly(ethylene oxide)- and Polyzwitterion-Based Thermoplastic Elastomers for Solid Electrolytes

In this article, ABA triblock copolymer (tri-BCP) thermoplastic elastomers with poly(ethylene oxide) (PEO) middle block and polyzwitterionic poly(4-vinylpyridine) propane-1-sulfonate (PVPS) outer blocks were synthesized. The PVPS-b-PEO-b-PVPS tri-BCPs were doped with lithium bis-(trifluoromethane-sulfonyl) imide (LiTFSI) and used as solid polyelectrolytes (SPEs). The thermal properties and microphase separation behavior of the tri-BCP/LiTFSI hybrids were studied. Small-angle X-ray scattering (SAXS) results revealed that all tri-BCPs formed asymmetric lamellar structures in the range of PVPS volume fractions from 12.9% to 26.1%. The microphase separation strength was enhanced with increasing the PVPS fraction (fPVPS) but was weakened as the doping ratio increased, which affected the thermal properties of the hybrids, such as melting temperature and glass transition temperature, to some extent. As compared with the PEO/LiTFSI hybrids, the PVPS-b-PEO-b-PVPS/LiTFSI hybrids could achieve both higher modulus and higher ionic conductivity, which were attributed to the physical crosslinking and the assistance in dissociation of Li+ ions by the PVPS blocks, respectively. On the basis of excellent electrical and mechanical performances, the PVPS-b-PEO-b-PVPS/LiTFSI hybrids can potentially be used as solid electrolytes in lithium-ion batteries.


Introduction
As lithium-ion batteries (LIBs) possess the advantages of high energy density, long lifespan, and high charging speed, they are becoming increasingly prevalent in recent years [1][2][3].Despite the increase in efficiency and convenience generated by LIBs, commercially used liquid electrolytes in LIBs may lead to some potential problems, such as dendrite formation, fire, and explosion [4][5][6].Utilizing solid polymer electrolytes (SPEs) in place of liquid electrolytes could be a prospective solution.SPEs have been the focal point of research advancements since their capability to dissolve lithium salts effectively was pioneered by Wright et al. [7], with a significant body of subsequent studies dedicated to the optimization of SPEs' architecture [8][9][10][11].SPEs with high shear moduli possess excellent processability and are able to inhibit dendrite growth [12][13][14].The predominant challenges associated with SPEs revolve around harmonizing ionic conductivity with mechanical strength and enhancing the suboptimal interfacial adherence between the electrode and electrolyte [15][16][17][18].Innovations such as the integration of novel lithium salts and anions, the copolymerization process, graft-modified polymers, and the formation of composites with inorganic ceramic fillers have shown promise in mitigating these issues [19].
With its excellent ability to dissolve lithium salts effectively and make mobility requisite for Li + ion transport, salt-doped poly(ethylene oxide) (PEO) serves as the most representative polymer electrolyte [20,21].There are several methods to modify homogeneous PEO materials for higher ionic conductivity and shear modulus, such as regulation of molecular weight [22], salt doping ratio [23], and temperature [24], but the trade-off between polymer chain mobility and stiffness makes it difficult to attain both excellent conductivity and mechanical strength [13,15].
Recently, block copolymers (BCPs) have been extensively studied due to their unique self-assembly structures at the nanoscale, which conduces to a combination of various distinctive properties [25,26].The connection of PEO with a reinforcing block can provide SPE materials with both ion transport channels and improved mechanical strength [27,28].Hillmyer's group reported a kind of BCP electrolyte material based on polymerizationinduced phase separation and found that the ionic conductivity of the material could reach 10 −3 S/cm at room temperature with its elastic modulus close to 1 GPa [16].However, among the majority of BCP materials studied, how to decouple conductivity with modulus completely still remains a problem [13,29], since introducing insulated blocks with better mechanical properties into the electrolytes usually has an adverse impact on ionic conductivity.For example, Balsara et al. showed that lithium bis-(trifluoromethane-sulfonyl) imide (LiTFSI)-doped poly(styrene)-b-PEO (PS-b-PEO) brought out enhanced modulus but restricted conductivity compared to PEO/LiTFSI [9,30,31].Notably, our group found that BCPs with double conductive phases that both constructing blocks are able to dissolve Li + ions as SPEs, such as poly(propylene monothiocarbonate)-b-PEO (PPMTC-b-PEO), could achieve synchronous enhancement of conductivity and modulus via regulating the microphase separation behavior of the double conductive phases [32,33].In our previous work, we systematically studied the effects of phase structure, grain size, and interphase on the conductivity of block copolymer electrolytes with double-conductive phases [32][33][34][35].
In the past few years, zwitterions and polyzwitterions have been extensively applied for gel polymer electrolytes (GPEs) or SPEs in LIBs [36][37][38][39].Zwitterions, such as sulfobetaine and carboxybetaine, contain covalently bonded cation and anion in a single molecule, while polyzwitterions represent polymers with repeating units bearing zwitterions [40,41].Ionic conductivity studies on polyzwitterion/salt systems were carried out by Manero et al., and they found that the conductivity of the systems followed the Arrhenius equation [42].Segalman and coworkers proposed semicrystalline polymeric zwitterionic (PZI) electrolytes with superionic lithium transport [43].Unlike the classical vehicular conduction mechanism in polyether and polymeric ionic liquid (PIL) electrolytes [44,45], lithium ion transport in these PZI electrolytes existed in two distinctive circumstances: The amorphous phase led to vehicular motion like traditional SPEs, and the ordered crystalline structure of pendant ZI groups enabled superionic transport similar to inorganic solid-state electrolytes, where Li + ions diffused nearly one order of magnitude more quickly than vehicular motion.Decoupling of ion transport with polymer segmental arrangement and size-selective ion motion for Li + ions facilitated by ordered lattices in the system resulted in high ionic conductivity and lithium transfer number.Macfarlane et al. introduced zwitterion in place of ionic liquid as a plasticizer into polymer electrolytes [46], and the conductivity and diffusion of lithium ions were significantly improved.They postulated that the oleophobic nature of zwitterion could enhance the mobility of Li + ions by providing a polar medium.Yoshizawa-Fujita designed a series of oligoether/zwitterion diblock copolymers and found the ionic conductivity of the SPEs to be maintained even at a high salt doping ratio [47].They proposed that the aggregation of dissociated ions was hindered by the polar zwitterion structure.Further implementation of these SPEs in cathode coatings for LIBs showed that these copolymers exhibited a substantial electrochemical stabilization window and preserved stable discharge capacities over successive cycles.
According to the strong intramolecular and intermolecular interactions of zwitterion in bulk, the zwitterion phase in zwitterion-containing copolymers presents enormous immiscibility with the other non-charged components [48,49].The bulk solidity below the glass transition temperature (T g ) makes it possible that the polyzwitterion phase serves as physical cross-linking points, thus enhancing the mechanical strength of the materials [50].Beyer and Long compared the storage moduli of n-butyl acrylate-based zwitterionomers and ionomers [51].They observed well-defined microphase separation and a rubbery plateau in zwitterionomers only when zwitterion content reached a certain amount.
In this work, ABA triblock copolymers (tri-BCPs) composed of poly(4-vinylpyridine) propane-1-sulfonate (PVPS) (A-block) and PEO (B-block) were used as SPE for LIBs for the purpose of simultaneous improvement in conductivity and mechanical performance.In addition to providing stiffness, the PVPS blocks can also dissociate and dissolve lithium salt, thus enabling the formation of double conductive phases in this type of ABA tri-BCP.The ionic conductivity and mechanical strength of the block copolymer solid electrolytes (BCPSEs), PVPS-b-PEO-b-PVPS/LiTFSI, with different compositions and doping ratios were investigated.It was observed that some of the electrolytes attained ionic conductivities and storage moduli higher than the PEO/LiTFSI blends.These electrically and mechanically enhanced SPEs are expected to inform the design of PEO-based electrolytes in LIBs in the future.

Synthesis of PVPS
in bulk, the zwi erion phase in zwi erion-containing copolymers presents enormous miscibility with the other non-charged components [48,49].The bulk solidity below glass transition temperature (Tg) makes it possible that the polyzwi erion phase serve physical cross-linking points, thus enhancing the mechanical strength of the mate [50].Beyer and Long compared the storage moduli of n-butyl acrylate-based zwi erio mers and ionomers [51].They observed well-defined microphase separation and a bery plateau in zwi erionomers only when zwi erion content reached a certain amo In this work, ABA triblock copolymers (tri-BCPs) composed of poly(4-vinylpyrid propane-1-sulfonate (PVPS) (A-block) and PEO (B-block) were used as SPE for LIBs the purpose of simultaneous improvement in conductivity and mechanical performa In addition to providing stiffness, the PVPS blocks can also dissociate and dissolve lith salt, thus enabling the formation of double conductive phases in this type of ABA tri-B The ionic conductivity and mechanical strength of the block copolymer solid electrol (BCPSEs), PVPS-b-PEO-b-PVPS/LiTFSI, with different compositions and doping ra were investigated.It was observed that some of the electrolytes a ained ionic condu ities and storage moduli higher than the PEO/LiTFSI blends.These electrically and chanically enhanced SPEs are expected to inform the design of PEO-based electrolyte LIBs in the future.

Preparation of Polymer/LiTFSI Hybrids
A certain amount of PVPSn-b-PEO210-b-PVPSn (or PEO210) and LiTFSI were dis in TFEA and stirred for 12 h to obtain homogeneous solutions.After being dried dynamic vacuum at room temperature for 24 h, the above blends were placed in a v oven for 48 h at 60 °C.Finally, the products were collected and stored in the glove an atmosphere of nitrogen.Doping ratio (r) is defined as the molar ratio of Li + ions sum of EO units and sulfonic acid units, both of which have the ability to comple Li + ions, i.e., r = [Li + ]/([EO] + [VPS]).

Characterizations
The composition of P4VP-b-PEO-b-P4VP tri-BCPs was determined by 1 H-NM Bruker DMX 400 (400 MHz) (Bruker Corporation, MA, USA) utilizing deuterated c form (CDCl3) as solvent.Relative molecular weight and polydispersity of PEO and b-PEO-b-P4VP were measured by gel permeation chromatography (GPC) (Waters C ration, MA, USA) on a Waters system with DMF as eluent and polystyrene (PS) as ards for calibration.The flow rate of DMF was kept at 1 mL/min while the test tempe was set at 40 °C.Fourier-transform infrared (FTIR) spectra were collected from a N 6700 spectrometer (Thermo Fisher Scientific Inc., MA, USA) with a resolution of Differential scanning calorimetry (DSC) was carried out on a TA DSC25 (TA Instru MA, USA) instrument to characterize the crystallization behavior and glass transitio perature (Tg) of the samples.The tests were performed with heating and cooling r 10 °C/min under nitrogen.Temperature-variable small-angle X-ray sca ering (SAX periments were operated at beamline BL16B1 (Shanghai Synchrotron Radiation F (SSRF), Shanghai, China) .Two-dimensional SAXS pa erns (2D-SAXS) were record a Pilatus 2M detector (Dectris Ltd, Baden, Swi erland) and transformed into one-d sional profiles with FIT2D software (h ps://www.esrf.fr/computing/scientific/FISamples were annealed for 24 h at 120 °C and stepwise cooled to room temperatur

Preparation of Polymer/LiTFSI Hybrids
A certain amount of PVPS n -b-PEO 210 -b-PVPS n (or PEO 210 ) and LiTFSI were dissolved in TFEA and stirred for 12 h to obtain homogeneous solutions.After being dried under dynamic vacuum at room temperature for 24 h, the above blends were placed in a vacuum oven for 48 h at 60 • C. Finally, the products were collected and stored in the glove box in an atmosphere of nitrogen.Doping ratio (r) is defined as the molar ratio of Li + ions to the sum of EO units and sulfonic acid units, both of which have the ability to complex with Li + ions, i.e., r = [Li + ]/([EO] + [VPS]).

Characterizations
The composition of P4VP-b-PEO-b-P4VP tri-BCPs was determined by 1 H-NMR with Bruker DMX 400 (400 MHz) (Bruker Corporation, Billerica, MA, USA) utilizing deuterated chloroform (CDCl 3 ) as solvent.Relative molecular weight and polydispersity of PEO and P4VP-b-PEO-b-P4VP were measured by gel permeation chromatography (GPC) (Waters Corporation, Milford, MA, USA) on a Waters system with DMF as eluent and polystyrene (PS) as standards for calibration.The flow rate of DMF was kept at 1 mL/min while the test temperature was set at 40 • C. Fourier-transform infrared (FTIR) spectra were collected from a Nicolet 6700 spectrometer (Thermo Fisher Scientific Inc., Waltham, MA, USA) with a resolution of 1 cm −1 .Differential scanning calorimetry (DSC) was carried out on a TA DSC25 (TA Instruments, Wakefield, MA, USA) instrument to characterize the crystallization behavior and glass transition temperature (T g ) of the samples.The tests were performed with heating and cooling rates of 10 • C/min under nitrogen.Temperature-variable smallangle X-ray scattering (SAXS) experiments were operated at beamline BL16B1 (Shanghai Synchrotron Radiation Facility (SSRF), Shanghai, China).Two-dimensional SAXS patterns (2D-SAXS) were recorded by a Pilatus 2M detector (Dectris Ltd., Baden, Switzerland) and transformed into one-dimensional profiles with FIT2D software (https://www.esrf.fr/computing/scientific/FIT2D/ accessed on 20 March 2024).Samples were annealed for 24 h at 120 • C and stepwise cooled to room temperature prior to SAXS testing.The wavelength of the X-ray was 1.24 Å, and the distance between the sample and the detector was 1920 mm.The average exposure time of the samples was 20 s.The scattering vector of the SAXS curves was calibrated with silver behenate.Temperature-variable rheological measurements were performed on a HAAKE RS 6000 rheometer (Thermo Fisher Scientific Inc., MA, USA) using 20 mm diameter parallel plates with a 1 mm gap between the plates.Temperature sweeps with a frequency of 1 Hz between 30 and 100 • C were collected within the linear viscoelastic regime at a heating rate of 2 • C/min under nitrogen.Before the rheological tests, the samples were thermally pressed into films with a thickness of 1 mm and cooled down to room temperature under relatively high pressure.The impedance spectroscopy of the polymer electrolyte films was recorded by an electrochemical workstation (CHI660E, CH Instruments, Inc., Bee Cave, TX, USA) under nitrogen with a frequency range of 1 MHz to 1 Hz and a fixed amplitude of 0.05 V.After being annealed at 120 • C for 24 h and cooled to room temperature, the electrolyte films were sandwiched between two stainless steel electrodes and a Teflon washer.The resistance that originated from ion transport in the polymer electrolytes was determined by the local minimum in the Nyquist plot of the impedance.The conductivities (σ) of the electrolytes were calculated by the equation σ = L/(R•S), where L, R, and S represent the electrolyte thickness, resistance, and area, respectively.

Microphase Separation Behavior
Figure 1 shows the SAXS profiles of PVPS n -b-PEO 210 -b-PVPS n tri-BCPs and PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids.It is found that, above the melting temperature (T m ) of PEO, all the neat tri-BCPs exhibit ordered lamellar structure as indicated by the relative position of higher-order peaks (q) and the primary peak (q*) (q: q* = 1: 2: 3:. ..) in SAXS profiles (Figure 1a).Notably, for traditional non-charged diblock copolymers, only when the volume fraction of a phase reaches 40% to 60% can lamellar structure be formed [53], while in our samples, the volume fractions of PVPS in lamella-forming samples are far below 40%.This is because introducing Coulombic interaction into BCPs may shift the symmetry of the phase diagram, and the lamellar structure formed at a low content of charged phase is a consequence of physical crosslinking among the polyzwitterion blocks [48,49].With the increase in zwitterionic PVPS content, most samples present a reduced peak width and more high-order peaks, indicating stronger phase separation.
to SAXS testing.The wavelength of the X-ray was 1.24 Å, and the distance betwee sample and the detector was 1920 mm.The average exposure time of the samples w s.The sca ering vector of the SAXS curves was calibrated with silver behenate.Tem ture-variable rheological measurements were performed on a HAAKE RS 6000 rheom (Thermo Fisher Scientific Inc. , MA, USA) using 20 mm diameter parallel plates wit mm gap between the plates.Temperature sweeps with a frequency of 1 Hz betwee and 100 °C were collected within the linear viscoelastic regime at a heating rate of 2 °C under nitrogen.Before the rheological tests, the samples were thermally pressed into with a thickness of 1 mm and cooled down to room temperature under relatively pressure.The impedance spectroscopy of the polymer electrolyte films was recorde an electrochemical workstation (CHI660E, CH Instruments, Inc. , TX, USA) under nitr with a frequency range of 1 MHz to 1 Hz and a fixed amplitude of 0.05 V.After b annealed at 120 °C for 24 h and cooled to room temperature, the electrolyte films sandwiched between two stainless steel electrodes and a Teflon washer.The resis that originated from ion transport in the polymer electrolytes was determined by the minimum in the Nyquist plot of the impedance.The conductivities (σ) of the electro were calculated by the equation σ = L/(R•S), where L, R, and S represent the electr thickness, resistance, and area, respectively.

Microphase Separation Behavior
Figure 1 shows the SAXS profiles of PVPSn-b-PEO210-b-PVPSn tri-BCPs and PVP PEO210-b-PVPSn/LiTFSI hybrids.It is found that, above the melting temperature (T PEO, all the neat tri-BCPs exhibit ordered lamellar structure as indicated by the rel position of higher-order peaks (q) and the primary peak (q*) (q: q* = 1: 2: 3:…) in S profiles (Figure 1a).Notably, for traditional non-charged diblock copolymers, only w the volume fraction of a phase reaches 40% to 60% can lamellar structure be formed while in our samples, the volume fractions of PVPS in lamella-forming samples ar below 40%.This is because introducing Coulombic interaction into BCPs may shif symmetry of the phase diagram, and the lamellar structure formed at a low conte charged phase is a consequence of physical crosslinking among the polyzwi erion b [48,49].With the increase in zwi erionic PVPS content, most samples present a red peak width and more high-order peaks, indicating stronger phase separation.In contrast, as the doping ratio rises, the ordering degree of the microphase-sepa structures becomes lower.Hybrids at different doping ratios show ill-defined struc at room temperature, as their SAXS profiles (Figure 1b-d) show no higher-order pea higher-order peaks with uncharacteristic proportional position relations to the pri In contrast, as the doping ratio rises, the ordering degree of the microphase-separated structures becomes lower.Hybrids at different doping ratios show ill-defined structures at room temperature, as their SAXS profiles (Figure 1b-d) show no higher-order peaks or higher-order peaks with uncharacteristic proportional position relations to the primary peaks.Homogeneous structures are even formed in PVPS 3.1 -b-PEO 210 -b-PVPS 3.1 /LiTFSI hy-brids at doping ratios of 1/12 and 1/6, as indicated by their flat SAXS profiles (Figure 1c,d).This result is related to the competitive distribution of lithium salt in different blocks, as proved by the FTIR spectra shown in Figure S4.Lithium salt is first distributed in the PEO phase, leading to the charged characteristic of the PEO block, improved similarity with the PVPS block, and decreased microphase separation strength.The shoulder peaks superposed on the primary scattering peaks observed at the doping ratio of 1/16 are attributed to PEO crystals, which will disappear after the fusion of PEO crystals (Figure S5).
Temperature-variable SAXS experiments were carried out for PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids at r = 1/16, among which n corresponds to 4.5, 6.2, and 7.4, respectively.In Figure S5, it is observed that the scattering vector ratio of the primary and higher-order peaks remains 1:2 at the temperatures above the melting of PEO crystal, suggesting that these hybrids maintain a lamellar structure.
The effective Flory Huggins parameter (χ eff ) between PEO and PVPS at the doping ratio 1/16 was obtained by fitting the disordered scattering peak of PVPS 3.1 -b-PEO 210 -b-PVPS 3.1 /LiTFSI hybrids in terms of the theory developed by Leibler [54][55][56].It is found that χ eff of this hybrid is 0.51 at 30 • C (Figure S6), much larger than 0.09 reported for PS-b-PEO/LiTFSI hybrids at the same doping ratio and temperature (detailed formula and calculation are given in Supplementary Materials) [30] and 0.092 for PEO 114 -b-P4VP 27 BCP at 60 • C [57].The strong incompatibility between PEO and PVPS accounts for the maintenance of the ordered structure, which ensures the formation of physical crosslinking points in the thermoplastic elastomers.

Thermal Properties
The thermal behaviors of PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids were characterized by DSC (detailed information is given in Table S2).As illustrated in Figure 2, a glass transition at low temperature and an endothermic peak are observed for each sample, while a cold crystallization process was seen in some specific samples.The endothermic peaks are ascribed to the melting of PEO.The crystallinity of PEO given in Table S2 was calculated based on the melting enthalpy, and it was found to decrease with the doping ratio.Notably, when the doping ratio is raised to 1/6, the crystallinity of PEO decreases to below 5%.As a result, the impact of crystallization on the subsequent experiments operated above r.t. for the samples with r = 1/6 can be ignored.
Materials 2024, 17, x FOR PEER REVIEW 6 peaks.Homogeneous structures are even formed in PVPS3.1-b-PEO210-b-PVPS3.1/LiTFS brids at doping ratios of 1/12 and 1/6, as indicated by their flat SAXS profiles (Figure 1 This result is related to the competitive distribution of lithium salt in different block proved by the FTIR spectra shown in Figure S4.Lithium salt is first distributed in the phase, leading to the charged characteristic of the PEO block, improved similarity the PVPS block, and decreased microphase separation strength.The shoulder peak perposed on the primary sca ering peaks observed at the doping ratio of 1/16 ar tributed to PEO crystals, which will disappear after the fusion of PEO crystals (Figur Temperature-variable SAXS experiments were carried out for PVPSn-b-PEO PVPSn/LiTFSI hybrids at r = 1/16, among which n corresponds to 4.5, 6.2, and 7.4, re tively.In Figure S5, it is observed that the sca ering vector ratio of the primary and hi order peaks remains 1:2 at the temperatures above the melting of PEO crystal, sugge that these hybrids maintain a lamellar structure. The effective Flory Huggins parameter (χeff) between PEO and PVPS at the do ratio 1/16 was obtained by fi ing the disordered sca ering peak of PVPS3.1-b-PEOPVPS3.1/LiTFSIhybrids in terms of the theory developed by Leibler [54][55][56].It is found χeff of this hybrid is 0.51 at 30 °C (Figure S6), much larger than 0.09 reported for PEO/LiTFSI hybrids at the same doping ratio and temperature (detailed formula and culation are given in Supplementary Materials) [30] and 0.092 for PEO114-b-P4VP27 BC 60 °C [57].The strong incompatibility between PEO and PVPS accounts for the ma nance of the ordered structure, which ensures the formation of physical crosslin points in the thermoplastic elastomers.

Thermal Properties
The thermal behaviors of PVPSn-b-PEO210-b-PVPSn/LiTFSI hybrids were chara ized by DSC (detailed information is given in Table S2).As illustrated in Figure 2, a transition at low temperature and an endothermic peak are observed for each sam while a cold crystallization process was seen in some specific samples.The endothe peaks are ascribed to the melting of PEO.The crystallinity of PEO given in Table S2 calculated based on the melting enthalpy, and it was found to decrease with the do ratio.Notably, when the doping ratio is raised to 1/6, the crystallinity of PEO decreas below 5%.As a result, the impact of crystallization on the subsequent experiments ated above r.t. for the samples with r = 1/6 can be ignored.respectively.The T g s observed in Figure 2 are close to those of PEO, so they are assigned to the PEO-rich phase in the PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids.After introducing PVPS block into the system, the T g s of the PEO-rich phase are increased in most cases compared with pure PEO homopolymers.It is found that, with increasing the volume fraction of PVPS, the T g becomes lower at first and then increases.Two aspects account for such a trend.When the content of PVPS is lower, the phase separation between PEO and PVPS is incomplete, along with a weaker spatial confinement effect on PEO segments, but there are more rigid PVPS segments in the PEO-rich phase.On the other hand, the degree of microphase separation is high at a larger volume fraction of PVPS, resulting in a lower PVPS content in the PEO-rich phase but a stronger spatial restriction on the segmental motion of PEO.As the doping ratio increases from 1/16 to 1/6, T g of the PEO-rich phase in PVPS 7.4b-PEO 210 -b-PVPS 7.4 /LiTFSI hybrids increases on account of suppression of PEO segmental motion by disassociated LiTFSI salt.However, T g s of PVPS 4.5 -b-PEO 210 -b-PVPS 4.5 /LiTFSI and PVPS 6.2 -b-PEO 210 -b-PVPS 6.2 /LiTFSI hybrids first decrease then increase with increasing salt content, while it takes a monotonous uptrend in PEO/LiTFSI hybrids.The phenomenon observed in the above tri-BCP/LiTFSI hybrids is ascribed to the enhancement in dissociation of LiTFSI by introducing polyzwitterion blocks, and such a downward trend in T g s has also been reported in oligoether/zwitterion diblock copolymers doped with LiTFSI [47].
Changes in crystallization and glass transition behaviors have a significant impact on the segmental motion of PEO chains.Lower crystallinity and T g of PEO correspond to better mobility and less stiffness of the polymer chain, which is beneficial for the increase in conductivity [20].C ranges from 10 0 to 10 3 Pa and decreases with increasing temperature.As the doping ratio increases, the initial storage modulus of PEO/LiTFSI hybrids drops at first and then becomes a little larger.This originates from two opposite aspects.On the one hand, salt doping restricts the crystallizability of PEO, thus impairing its mechanical properties.On the other hand, salt also serves as a crosslinking point for the homogeneous melt of PEO, which will enhance the modulus.

Rheological Properties
ume fraction of PVPS, the Tg becomes lower at first and then increases.Two aspects account for such a trend.When the content of PVPS is lower, the phase separation between PEO and PVPS is incomplete, along with a weaker spatial confinement effect on PEO segments, but there are more rigid PVPS segments in the PEO-rich phase.On the other hand, the degree of microphase separation is high at a larger volume fraction of PVPS, resulting in a lower PVPS content in the PEO-rich phase but a stronger spatial restriction on the segmental motion of PEO.As the doping ratio increases from 1/16 to 1/6, Tg of the PEOrich phase in PVPS7.4-b-PEO210-b-PVPS7.4/LiTFSI hybrids increases on account of suppression of PEO segmental motion by disassociated LiTFSI salt.However, Tgs of PVPS4.5-b-PEO210-b-PVPS4.5/LiTFSI and PVPS6.2-b-PEO210-b-PVPS6.2/LiTFSI hybrids first decrease then increase with increasing salt content, while it takes a monotonous uptrend in PEO/LiTFSI hybrids.The phenomenon observed in the above tri-BCP/LiTFSI hybrids is ascribed to the enhancement in dissociation of LiTFSI by introducing polyzwi erion blocks, and such a downward trend in Tgs has also been reported in oligoether/zwi erion diblock copolymers doped with LiTFSI [47].
Changes in crystallization and glass transition behaviors have a significant impact on the segmental motion of PEO chains.Lower crystallinity and Tg of PEO correspond to be er mobility and less stiffness of the polymer chain, which is beneficial for the increase in conductivity [20].

Rheological Properties
Figure 3 shows the variation of storage modulus (G′) with temperature for the PVPSnb-PEO210-b-PVPSn/LiTFSI and PEO210/LiTFSI hybrids at different doping ratios.The initial G′ of PEO210/LiTFSI hybrids at 30 °C ranges from 10 0 to 10 3 Pa and decreases with increasing temperature.As the doping ratio increases, the initial storage modulus of PEO/LiTFSI hybrids drops at first and then becomes a li le larger.This originates from two opposite aspects.On the one hand, salt doping restricts the crystallizability of PEO, thus impairing its mechanical properties.On the other hand, salt also serves as a crosslinking point for the homogeneous melt of PEO, which will enhance the modulus.All the PVPSn-b-PEO210-b-PVPSn/LiTFSI hybrids exhibit higher G′ values than the PEO210/LiTFSI hybrids due to the reinforcement of the PVPS phase.Hybrids with a larger fraction of the PVPS block exhibit a higher G′ at the same doping ratio.The value of G′ for PVPS7.4-b-PEO210-b-PVPS7.4/LiTFSI hybrid at r = 1/6 can reach 3 × 10 5 Pa, which is at least 10 4 times higher than that of PEO210/LiTFSI hybrid at the same doping ratio.It is also observed that, with increasing temperature, the modulus of some tri-BCP hybrids first maintains a plateau in the low temperature range and then decreases gradually at higher temperatures.The turning point shifts to a higher temperature as fPVPS in the tri-BCPs increases.Since the temperature corresponding to the turning point can be higher than the Tm of PEO and no order-to-disorder transition is observed around the turning point (Figure S7), the decrease of G′ may be a ributed to the pulling-out of partial PVPS blocks from All the PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids exhibit higher G ′ values than the PEO 210 /LiTFSI hybrids due to the reinforcement of the PVPS phase.Hybrids with a larger fraction of the PVPS block exhibit a higher G ′ at the same doping ratio.The value of G ′ for PVPS 7.4 -b-PEO 210 -b-PVPS 7.4 /LiTFSI hybrid at r = 1/6 can reach 3 × 10 5 Pa, which is at least 10 4 times higher than that of PEO 210 /LiTFSI hybrid at the same doping ratio.It is also observed that, with increasing temperature, the modulus of some tri-BCP hybrids first maintains a plateau in the low temperature range and then decreases gradually at higher temperatures.The turning point shifts to a higher temperature as f PVPS in the tri-BCPs increases.Since the temperature corresponding to the turning point can be higher than the T m of PEO and no order-to-disorder transition is observed around the turning point (Figure S7), the decrease of G ′ may be attributed to the pulling-out of partial PVPS blocks from the physical crosslinking domains under dynamic shearing.The physical crosslinking domains become more stable at a higher f PVPS , and as a consequence, the PVPS 7.4 -b-PEO 210b-PVPS 7.4 /LiTFSI hybrids even keep nearly constant moduli in the temperature range studied (30-100 • C).The relatively high and constant moduli of the PVPS 7.4 -b-PEO 210 -b-PVPS 7.4 /LiTFSI hybrids in a broad temperature range are advantageous to the processing and application of SPEs for LIBs with good safety.It is reported that lithium dendrites can be suppressed when the shear modulus of the separator (approximately 6 GPa) is 1.8 times higher than that of Li metal (4.9 GPa) [60].Although the overall moduli of the PVPS-b-PEOb-PVPS/LiTFSI hybrids are at the magnitude of 10 5 Pa, due to the microphase-separated structure formed in the hybrids, the growth of lithium dendrites cannot bypass the PVPS microdomains, and it will be stopped when meeting the glassy PVPS microdomains with a high modulus.

Ionic Conductivity
The electrical performances of PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids were characterized by the impedance spectrum.Figure 4  /LiTFSI exhibits ionic conductivities comparable to PEO 210 /LiTFSI.This may be due to the relative enrichment of LiTFSI in the PEO phase, which is frequently observed in the hybrids of salt and BCPs where both blocks can complex with salt, especially at low doping ratios [33,34,61].With further increasing the PVPS fraction in the tri-BCPs, the ionic conductivities of PVPS 6.  S2 shows that the minimal T g of PEO occurs in the PVPS 6.2 -b-PEO 210 -b-PVPS 6.2 /LiTFSI hybrids, suggesting a lower concentration of PVPS in the PEO-rich phase due to enhanced microphase separation.This implies that at this juncture, the limitation of chain segment motion is not the predominant influence on conductivity.Furthermore, the grain sizes resulting from microphase separation for each sample set, as detailed in Table S3, do not adequately justify the reduced conductivity observed at elevated PVPS content with low salt-doping ratios [62,63].It is postulated that with increased PVPS content, microphase separation becomes more pronounced and the phase interfaces are more defined.Consequently, at lower lithium salt concentrations, salts predominantly localize within the interstitial zones of the PEO phase, akin to the PS-b-PEO system [25].This distribution limits the efficacy of PVPS in facilitating salt dissociation, and the morphology effect and grain boundary effect culminate in actual conductivities that are less than theoretical predictions.In the hybrids of tri-BCP, the nominal doping ratio is denoted as r = [LiTFSI]/([EO] + [VPS]).Since the PEO block has stronger association ability toward Li + ions than the PVPS block, the salt concentration in the PEO phase of tri-BCPs hybrids is higher than that in PEO 210 /LiTFSI, leading to the higher conductivity of the former.We also notice that the ionic conductivities of PVPS 6.2 -b-PEO 210 -b-PVPS 6.2 /LiTFSI and PVPS 7.4 -b-PEO 210 -b-PVPS 7.4 /LiTFSI at 1/16 are quite low in the low temperature range.This can be attributed to the presence of un-melted PEO crystals at testing temperatures, as confirmed by their higher T m s of PEO (Figure 2 and Table S2).This can be attributed to the unique dipole nature of zwitterionic molecules, which probably induce the Li + ions to dissociate from the lithium salt.In the literature, it was also reported that the introduction of zwitterion or polyzwitterion into the electrolytes by blending [64] or random copolymerization [65] could improve the electrical performance.It should be noted that the effect of helping dissociate Li + ions becomes obvious only at high doping ratios and in tri-BCPs with high PVPS fractions, since at low doping ratios, there are few salts in the PVPS phase with weaker association ability.This also leads to the high ionic conductivities of PVPS 6.The Vogel-Tammann-Fulcher (VTF) equation was frequently utilized to describe the temperature dependence of the ionic conductivity of polymer electrolytes [66,67].It can be written as follows: ln where T 0 represents the reference temperature set as T g -50 °C, E a is the apparent activation energy for ion transport, A is a pre-factor, and R is the gas constant, which equals 8.314 J/(mol•K).When ln(σT 1/2 ) is plotted versus 1/(T-T 0 ), a linear relationship is acquired.The slope of the line corresponds to −E a /R, and the intercept corresponds to lnA.The plots of logarithmic ionic conductivity against 1/(T-T 0 ) for the hybrids are shown in Figure 5, and the calculated E a s are listed in Table S4.The obtained E a s in this work are comparable with the values (~10 kJ/mol) reported for other PEO-based SPEs [68,69].We notice that at low PVPS fractions, E a s increases as the doping ratio increases, while for PVPS 6.It is counter-intuitive that E a s decreases with increasing doping ratio after r reaches 1/12, since restriction of chain segment motion resulting from superfluous lithium salt can be verified by increasing T g s (Table S2).This abnormal phenomenon is attributed to different salt distribution situations.For hybrids with low PVPS contents, lithium salt is mainly located in the PEO-rich phase, but at high PVPS fractions, PVPS blocks help with the dissociation of LiTFSI, thus decreasing E a s.S5 summarizes the ionic conductivity and storage modulus of PVPS-b-PEO-b-PVPS/LiTFSI hybrids and other BCP-based SPEs reported in the literature.As we can see, the PVPS-b-PEO-b-PVPS/LiTFSI hybrids in this work exhibit a better balance in ionic conductivity and moduli as compared with most other BCP electrolyte materials.This shows that the integration of PVPS offers valuable insights for the development of novel SPEs for LIBs.

Conclusions
In summary, the solid electrolytes of LiTFSI-doped PVPS-b-PEO-b-PVPS ABA tri-BCP thermoplastic elastomers were successfully prepared.Asymmetric lamellar microphaseseparated structures were formed in all the PVPS-b-PEO-b-PVPS tri-BCPs studied.By increasing the f PVPS in the tri-BCPs, the lamellar structure becomes more ordered, while salt-doping weakens the tendency toward microphase separation.The melting temperature and glass transition temperature of the hybrids were influenced by the f PVPS , the spatial confinement of the microphase-separated structure, and the doping ratio.Due to the physical crosslinking domains formed by the glassy PVPS blocks, the moduli of the PVPS-b-PEO-b-PVPS/LiTFSI hybrids are greatly improved as compared with the PEO/LiTFSI hybrids.Moreover, the PVPS-b-PEO-b-PVPS/LiTFSI hybrids can outperform the PEO/LiTFSI hybrids in ionic conductivity due to the assistance of the PVPS blocks in the dissociation of Li + ions.As a result, simultaneous improvement of mechanical properties and ionic conductivity can be achieved by the introduction of PVPS at both ends of PEO, which makes the PVPS-b-PEO-b-PVPS/LiTFSI hybrids have potential application in LIBs as solid electrolytes.
-b-PEO-b-PVPS tri-BCPs PVPS-b-PEO-b-PVPS tri-BCPs were synthesized by reversible addition-fragmentation chain transfer (RAFT) polymerization.First, esterification of PEO with TTCA was carried out in the presence of oxalyl chloride dissolved in CH 2 Cl 2 , and the CTA-PEO-CTA double-ended macromolecular chain transfer agent was prepared.Next, a series of poly(4-vinylpyridine)b-poly(ethylene oxide)-b-poly(4-vinylpyridine) (P4VP-b-PEO-b-P4VP) ABA triblock BCPs were synthesized via RAFT polymerization of 4-VP in DMF.1,3-propanesultone was then added for further modification of the pyridine group in TFEA.The detailed synthesis process and characterization results of the polymers are provided in the Supplementary Materials.Scheme 1 shows the synthesis route of PVPS-b-PEO-b-PVPS tri-BCPs.Table

Table 1 . 1 a
Details for PVPS-b-PEO-b-PVPS tri-BCPs.The number of repeating units was determined by 1 H-NMR of P4VP-b-PEO-b-P4VP.b The n average molecular weight is calculated by 1 H-NMR spectra.c Polydispersity of P4VP-b-PEO-b Ð = Mw/Mn obtained from GPC. d The volume fraction of PVPS is calculated on the basis of t sities of PEO (1.128 g/cm 3 ) and PVPS (1.16 g/cm 3 ) [48,52].

Figure 2 .
Figure 2. DSC 2nd heating curves of PEO 210 /LiTFSI and PVPS n −b−PEO 210 −b−PVPS n /LiTFSI with different doping ratios.(a) r = 1/16, (b) r = 1/12, and (c) r = 1/6.It is reported in the literature that the T g s of PEO and PVPS are −65 • C and 226 • C [58,59],respectively. The T g s observed in Figure2are close to those of PEO, so they are assigned to the PEO-rich phase in the PVPS n -b-PEO 210 -b-PVPS n /LiTFSI hybrids.After introducing PVPS block into the system, the T g s of the PEO-rich phase are increased in most cases compared with pure PEO homopolymers.It is found that, with increasing the volume fraction of PVPS, the T g becomes lower at first and then increases.Two aspects account for such a trend.When the content of PVPS is lower, the phase separation between PEO and PVPS is incomplete, along with a weaker spatial confinement effect on PEO segments, but there

Figure 3
Figure 3 shows the variation of storage modulus (G ′ ) with temperature for the PVPS nb-PEO 210 -b-PVPS n /LiTFSI and PEO 210 /LiTFSI hybrids at different doping ratios.The initial G ′ of PEO 210 /LiTFSI hybrids at 30• C ranges from 10 0 to 10 3 Pa and decreases with increasing temperature.As the doping ratio increases, the initial storage modulus of PEO/LiTFSI hybrids drops at first and then becomes a little larger.This originates from two opposite aspects.On the one hand, salt doping restricts the crystallizability of PEO, thus impairing its mechanical properties.On the other hand, salt also serves as a crosslinking point for the homogeneous melt of PEO, which will enhance the modulus.